Polymorphism of Li~2~Zn~3~
Pavlyuk, Volodymyr; Chumak, Ihor; Ehrenberg, Helmut; Acta Crystallographica Section B 68 (2012) 34–39; doi:10.1107/S0108768111053493

data_2105050
_publ_section_title
;
 Polymorphism of Li~2~Zn~3~
;
_journal_coeditor_code           BP5039
_journal_issue                   1
_journal_name_full               'Acta Crystallographica Section B'
_journal_page_first              34
_journal_page_last               39
_journal_paper_doi               10.1107/S0108768111053493
_journal_volume                  68
_journal_year                    2012
_chemical_formula_moiety         'Li0.62 Zn0.87'
_chemical_formula_sum            'Li0.62 Zn0.87'
_chemical_formula_weight         61.87
_space_group_IT_number           164
_symmetry_cell_setting           trigonal
_symmetry_space_group_name_Hall  '-P 3 2"'
_symmetry_space_group_name_H-M   'P -3 m 1'
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                120.00
_cell_formula_units_Z            6
_cell_length_a                   4.3528(14)
_cell_length_b                   4.3528(14)
_cell_length_c                   8.003(3)
_cell_measurement_reflns_used    1795
_cell_measurement_temperature    296(2)
_cell_measurement_theta_max      29.06
_cell_measurement_theta_min      2.55
_cell_volume                     131.32(8)
_computing_cell_refinement       'SAINT (Bruker, 2004)'
_computing_data_collection       'APEX2 (Bruker, 2004)'
_computing_data_reduction        'SAINT (Bruker, 2004)'
_computing_molecular_graphics    'Diamond (Brandenburg, 1999)'
_computing_publication_material  'SHELX-97 (Sheldrick, 1997)'
_computing_structure_refinement  'SHELXTL (Sheldrick, 2008)'
_computing_structure_solution    'SHELXTL (Sheldrick, 2008)'
_diffrn_ambient_temperature      296(2)
_diffrn_detector_area_resol_mean 25
_diffrn_measured_fraction_theta_full 0.975
_diffrn_measured_fraction_theta_max 0.975
_diffrn_measurement_device_type  'Bruker Kappa APEXII CCD area-detector'
_diffrn_measurement_method       '\f scans'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.1562
_diffrn_reflns_av_sigmaI/netI    0.0523
_diffrn_reflns_limit_h_max       5
_diffrn_reflns_limit_h_min       -5
_diffrn_reflns_limit_k_max       5
_diffrn_reflns_limit_k_min       -5
_diffrn_reflns_limit_l_max       10
_diffrn_reflns_limit_l_min       -10
_diffrn_reflns_number            1795
_diffrn_reflns_theta_full        29.06
_diffrn_reflns_theta_max         29.06
_diffrn_reflns_theta_min         2.55
_diffrn_standards_decay_%        0
_diffrn_standards_interval_count 0
_diffrn_standards_interval_time  0
_diffrn_standards_number         0
_exptl_absorpt_coefficient_mu    23.568
_exptl_absorpt_correction_T_max  0.623
_exptl_absorpt_correction_T_min  0.211
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   '(SADABS; Bruker, 2004)'
_exptl_crystal_colour            'metallic dark grey'
_exptl_crystal_density_diffrn    4.694
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       plate
_exptl_crystal_F_000             170.1
_exptl_crystal_size_max          0.07
_exptl_crystal_size_mid          0.06
_exptl_crystal_size_min          0.02
_refine_diff_density_max         1.855
_refine_diff_density_min         -1.079
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.266
_refine_ls_matrix_type           full
_refine_ls_number_parameters     19
_refine_ls_number_reflns         159
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.266
_refine_ls_R_factor_all          0.0805
_refine_ls_R_factor_gt           0.0575
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[\s^2^(Fo^2^)+(0.0669P)^2^+0.0000P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1271
_refine_ls_wR_factor_ref         0.1419
_reflns_number_gt                118
_reflns_number_total             159
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            bp5039.cif
_cod_data_source_block           Li2Zn3-HT
_cod_original_cell_volume        131.31(8)
_cod_database_code               2105050